| ||Format||Pages||Price|| |
|3||$44.00||  ADD TO CART|
|Hardcopy (shipping and handling)||3||$44.00||  ADD TO CART|
Significance and Use
3.1 This test method is used as a means of determining the quality of cemented carbide grade powders by measuring their sintered strength. It is performed on test specimens prepared to specified shape, dimensions, and surface finish; test specimens may be prepared from finished parts if size permits. There is no known standard material for this test method. The transverse rupture strength of cemented carbides is not a design value.
3.1.1 Most commercial cemented carbides have mechanical behavior that is best classified as brittle (negligible ductility). Fracture strengths are dependent on internal or surface flaws. Examples of incoherent internal flaws are macropores, Type B porosity (see Test Method ), and inclusions of foreign particles. Such flaws are randomly distributed spatially and in size within the sintered material. This imparts a statistical nature to any transverse rupture strength measurement.
3.1.2 The stress distribution in a beam in three-point loading is non-uniform. It increases linearly along the span to a maximum at the center, and varies linearly through any section from compression on the top to tension on the bottom. The maximum tensile stress therefore occurs at center span in the bottom most fibers of the sample, and is defined as the transverse rupture strength at failure. Failure is initiated at a random flaw site, which is most probably not coincident with the maximum stress. This imparts an additional statistical nature to transverse rupture strength measurements.
1.1 This test method covers the determination of the transverse rupture strength of cemented carbides.
1.2 The values stated in inch-pound units are to be regarded as the standard. The SI values in parentheses are provided for information only.
1.3 This standard does not purport to address the safety concerns, if any, associated with its use. It is the responsibility of the user of this standard to establish appropriate safety and health practices and determine the applicability of regulatory limitations prior to use.
2. Referenced Documents (purchase separately) The documents listed below are referenced within the subject standard but are not provided as part of the standard.
B276 Test Method for Apparent Porosity in Cemented Carbides
ISO StandardISO-3327 HardmetalsDetermination of Transverse Rupture Strength
ICS Number Code 77.160 (Powder metallurgy)
UNSPSC Code 31133703(Cemented carbide powdered metal and metal alloy)
|Link to Active (This link will always route to the current Active version of the standard.)|
ASTM B406-96(2015), Standard Test Method for Transverse Rupture Strength of Cemented Carbides, ASTM International, West Conshohocken, PA, 2015, www.astm.orgBack to Top